8. Intergranular Corrosion (IGC).
Localized attack at and adjacent to grain boundaries, with relatively little corrosion of the grains. The alloy, sensitive to IGC, disintegrates and/or loses its strength when exposed to environments.8.1 Causes of intergranular corrosionA. Segregation of impurities at the grain boundary ex) Fe in Al alloys.B. Enrichment of one of the alloying elements or depletion of one of these elements in the grain boundary areas.
8.2 Intergranular Corrosion of stainless steels and nickel based alloys
Exposed temperature : 425 oC to 815 oC
SensitizationThis results from the preferential attack of Cr- depleted zone due to precipitation of Cr23C6 at grain boundary.
Effects of % C on senitization time of 304
8.3 Weld Decay and Knifeline Attack(KLA) Fe-Cr alloy
An intergranular attack in welded structures. The weld decay zone is within the heat affected zone(HAZ) somewhat removed from the weld bead itself. At position B In Fig.3-29, the alloy is in the critical temperature range for sufficient time to produce sensitization. KLA is a highly localized form of IGC that occurs for only a few grain diameters immediately adjacent to the weld bead in Type 321 and 347 austenitic stainless steels.
8.4 Control of IGC Fe-Cr alloy1) Metallurgical measures : a) Solution annealing : heating the alloy to 1050 C where all Cr-carbides are dissolved, followed by rapid cooling.b) Low-carbon alloy modifications : lower the carbon content to below 0.03% for austenitic stainless steels(304L, 316L) or to below 50ppm for ferritic stainless steels.c) Stabilization treatment : add strong carbide former(Ti, Nb) in melt:Types 347 and 321 stainless steels.2) Environmental measures : lower acidity and less oxidizing conditions will generally reduce the susceptibility to IGC.
1) Oxalic acid test Fe-Cr alloy
Polishing of specimen Etch the specimen for 1.5 min. at 1.0 A/cm2 in oxalic acid Determine the type of surface morphology :
A. Single loop test
For 304 stainless steel in 0.5M H2SO4 + 0.01M KSCN solution in which the Ecorr is -400mV,SCE.a. Polarize the alloy to the passivation range or +200mV,SCE and hold there for 2 min.b. Reverse scan at 6V/hr (1.67mV/sec) to Ecorr. Obtain E vs. log (current) curve from which electric charge Q during the reactivation process is measured. The Q ( the shaded area under the reactivation peak) depends on the total area of the Cr-depleted zone.
c. A measure of sesitization : Pa = Q/GBA, Coul/cm2GBA(grain boundary area) is calculated from the following eq. GBA = As[ 5.095 10-3 exp(0.347x)], where As is the sample area in cm2 and x is the ASTM grain size at 100 magnification.
B. Double Loop Test Fe-Cr alloy
The testing solution, temperature and cell components are the same as those in the single loop test.a. Expose the specimen to the solution for about 2 min. to establish the Ecorr(-400mV,SCE).b. Polarize it anodically to the passivation range of + 300mV,SCE at a rate of 6V/hr.c. Reverse scan to the Ecorr at a rate of 6V/hr.d. Measure the maximum currents for each loop : Ia for the large anodic loop, and Ir for the smaller loop generated during reactivation. A measure of degree of sensitization = Ir/Ia
8.5 IGC of Other Alloys Fe-Cr alloy1) Ni-Cr alloys
• INCONEL600 (Ni-16Cr-9Fe) alloy fails by IGC and IGSCC in the caustic(alkaline) solutions that concentrate in the crevices.
2) Al alloys
• Al-Mg (5xxx) alloys : Mg2Al8 is active to the Al matrix.• Al-Mg-Zn (7xxx) alloys : MgZn2 is active to the Al matrix.• Al-Cu (2xxx) and Al-Zn-Mg-Cu(7xxx) alloys : The copper depleted zone adjacent to grain boundary precipitates (Al2Cu) is attacked anodically.
Condition of Standard EPR test Fe-Cr alloy
Severe General corrosion + pitting Low discriminating power for DOS
Too Severe test condition
Predicting IGSCC susceptibility of Alloy 600 using Modified EPR test.• Ref. M. K. Ahn et al. Corrosion 51(1995) p. 441 IGC & IGSCC : Corrosion damages occurred most frequently in alloy 600 steam generator tubes
Condition of Modified EPR test Fe-Cr alloy
DOS = Ir/Ia
Modified EPR Test Ir/Ia = f ( electrolyte, T, VSCAN)
• Selective Grain Boundary attack• High Discriminating power for DOS of alloy 600.
The Modified DL-EPR test gave a closer correlation to S Fe-Cr alloyIGSCC than the standard DL-EPR tests because the modified test attacks the deeper chromium-depleted region selectively, with the shallower chromium-depleted region remained immune.
Relationship between EPR test result and IGSCC susceptibility.
Stress vs. strain curves of alloy 600 aged at 700 oC
Comparison between the results of EPR tests and SIGSCC of alloy 600 aged at 700 oC